Laser Surface Modiication of Ti6Al4V-Cu for Improved Microhardness and Wear
Mutiu Folorunsho Erinoshoa*, Esther Titilayo Akinlabia, Sisa Pityanab, Gbadebo Owolabic
Received: February 03, 2017; Revised: May 02, 2017; Accepted: May 27, 2017
To modify the properties of Ti6Al4V alloy, Cu has been added to host an antimicrobial efect in
the revised alloy for marine application. The Laser Metal Deposition (LMD) process on the Ti6Al4V
alloy and Cu was been investigated for surface modiication in order to combat the problem of
biofouling in the marine industry. The investigations focused on the microstructural observations, micro-hardness measurements and dry sliding wear in the presence of 3 and 5 weight percents of Cu. The microstructure results showed that Widmanstätten microstructures were formed in all the samples and lose their robustness towards the fusion zone as a result of the transition of heat sink towards the substrate. The microhardness values of Ti6Al4V-3Cu and Ti6Al4V-5Cu alloys were greatly improved to 547±16 VHN0.5 and 519±54 VHN0.5 respectively. Furthermore, the behaviour of wear loss on the surface of the Ti6Al4V-Cu alloys exhibited great improvement as compared with the parent material.
Keywords: dry sliding wear, laser metal deposition, microstructure, micro-hardness measurements, Ti6Al4V-Cu alloy, wear loss
* e-mail: email@example.com
Titanium and its alloys are amongst the most important alloys of the advanced materials which are the key to improving performance in the aerospace and terrestrial systems1-3. The improvements in mechanical properties of the
titanium alloys have generally been accomplished through the addition alloying compound4-7. The alloying additions in titanium can be divided into three diferent classes. The α-stabilizers such as Aluminium which impact solid solution strengthening to titanium; the β-stabilizers such as
copper, chromium, vanadium, iron, niobium, molybdenum
and manganese. They serve to introduce the β-phase in the α-phase microstructural counterpart; and the neutral
additions such as tin and zirconium also contribute towards solid solution strengthening8. According to the structural
alloy hand book, most of these alloys have found restricted use in the mechanical engineering applications due to their
poor abrasive wear resistance, high coeicient of friction and
the fretting characteristics. These anomalies behaviour of
titanium alloys could be enhanced and modiied by treating
the surfaces with coatings9. Four main mechanisms have
been stipulated to improve the wear behaviour of titanium alloys and these are: increase in the hardness, inducing
compressive residual stress, reduction in the coeicient of
friction and increase in the surface roughness10. Titanium
nitride has been coated on copper and brass substrates
with an electroless nickel interlayers. The hardness of the composite was increased with the electroless nickel interlayer
thickness. The coeicient of friction was also increased with
an increase in the thickness of electroless nickel interlayer for both copper and brass substrates11. The wear behaviour
of teeth was evaluated with cast titanium alloys containing 3 weight percent of copper, 5 weight percent of copper and Ti6Al4V alloy containing 1 weight percent of copper and 4 weight percent of copper. Their results were compared with commercially pure (CP) titanium, Ti6Al4V alloy and gold alloy. The wear resistance of the CP Ti and Ti6Al4V with copper addition Cu were found to show better wear properties than the Ti and Ti6Al4V alloy. Gold alloy was also presented to have the best wear property. Conclusion was made that wear resistance was improved with the copper alloying and with the introduction of Ti/Ti2Cu eutectoid12.
The framework of this research work originates with an overview of the contingent works that have been carried out by famous authors and researchers from perspective and area of specialisation. Biofouling is a major dilemma for many materials when exposed to chemically aggressive sea water13.
It is the growth of micro-organisms at the interface of metal14,
and this problem has caused an increase in maintenance, fuel and downtime costs to the shipping industry15. 10 wt
% of Cu was added to Al and Ti, and the resulting sample is subjected to corrosion test in natural sea water. The presence of Cu improved the corrosion resistance of Al, and however, a Department of Mechanical Engineering Science, University of Johannesburg, Auckland Park
Kingsway Campus, Johannesburg, 2006, South Africa
b Council for Scientiic and Industrial Research, National Laser Centre, PO Box 375, Pretoria, 0001, South Africa
the addition of 5 wt % Ti also enhanced the passivation and good corrosion rate16. It was found that alloys containing
60-70 % Cu content attack marine growth. However, this Cu can be used in anodic production to form Cu ions (Cu2+) during oxidation. This is of high toxicity, and is efective
for destroying the marine organisms. An investigation was conducted using copper-sulphate solution in a reversible reaction; and this proved that the Cu2+ reduces both macro-
and micro-biological fouling17. In this present work, Cu
has been selected due to its antimicrobial property, and in addition, it is a naturally hygienic metal, which retards the growth of harmful germs. These properties have thus, made it ideal for brewing vessels18. Several anti-biofouling
agencies such as chemical, biological and mechanical
methods are in practice but their efects are not signiicant.
Natural source antifouls are considered as one of the best replacement options for the antifouling processes19. However,
the motivation for this work is to modify and improve the surface of Ti6Al4V alloy with the addition of Cu for better microhardness and wear resistance properties through the laser metal deposition (LMD) process for marine application. The novelty of this work is the introduction of 3 weight percent (wt %) of Cu to titanium alloy (Ti6Al4V-3Cu) and 5 wt % of Cu to Ti6Al4V alloy (Ti6Al4V-5Cu) respectively, for the purpose of reducing the problem of biofouling in the marine industries. The parameters used in this study were selected from the preliminary studies and the chosen deposited Ti6Al4V-Cu alloys for characterization were of good bonding and surface roughness.
2. Experimental Structure and Techniques
The main laser deposition experiment was conducted at
the Council of Scientiic and Industrial Research, Pretoria, South Africa, CSIR. The equipment used was Ytterbium iber
laser system equipment (YLS-2000-TR) and function at a maximum power of 2 kW. Figure 1 shows a typical Kuka robot with a nozzle attached to the laser head performing LMD operation.
Two powders used for this research were Ti6Al4V and Cu powders and having particle sizes varying between 100
and 200 µm. The two powders were fed from two diferent hoppers and their lows were assisted with the aid of an argon
Figure 1. Typical Kuka robot.
Table 1. Experimental matrix.
Sample Name Laser Power (W) Scanning Speed (m/min) Copper Wt.% (%)
Powder Flow rate (rpm) Gas Flow rate (l/min)
Ti6Al4V Cu Ti6Al4V Cu
Z1 1200 0.7 5 2.4 0.1 3 1
Z2 1600 0.3 3 2.5 0.1 3 1
Z3 1200 0.3 5 2.4 0.1 3 1
Z4 1400 0.3 5 2.4 0.1 3 1
Z5 1600 0.3 5 2.4 0.1 3 1
Ti6Al4V 1600 0.3 0 2.4 Nil 3 Nil
gas (carrier gas). The argon gas was also supplied to provide a shield during the deposition to prevent oxygen contamination on the deposited alloys. A 99.6 % solid rectangular plate of Ti6Al4V alloy dimensioned with (102 X 102 X 7.45) mm3
was used as the substrate. The substrate was grit-blasted prior to deposition to remove surface contaminants and to
prepare the surface for irm metallographic bonding between
the alloys formed. Table 1 depicts the process parameters used for the experiment.
The beam diameter, the track length and the standof
distance were set at 4 mm, 5 mm and 12 mm respectively. All the samples were prepared following the procedures of grinding, polishing and etching according to E3-11 ASTM standard20.
According to the guidelines listed in the Struers application note of metallurgical preparation of titanium, the Kroll’s reagent was prepared for the etchant with (100 ml H2O, 2-3 ml HF and 4-6 ml HNO3)21. Each sample was etched for 10
-15 seconds, cleaned with ethanol, rinsed under running water
and dried of prior to Scanning Electron Microscope (SEM)
and Cu powders. Figures 2 a-b show the morphologies of Ti6Al4V and Cu powders.
The morphologies of both the Ti6Al4V and Cu powders were spherical in shape. The particle size of Ti6Al4V was observed to be equiaxed and the surfaces were smooth with satellites (dust particles) agglomerated scantily to the bigger particles. The particle sizes of Cu were also observed to be equiaxed in morphology and showed denser and immense faces compared to Ti6Al4V alloy powders.
2.2. Hardness test
Microhardness tests were performed on both the cross section and the surface of the substrate; and each of the deposited Ti6Al4V-Cu alloys on a Vickers hardness machine Zwick/Roell. A load of 500 g and a dwell time of 15seconds were used throughout the hardness test according E384 -11e1 ASTM standard22.
2.3. Wear test and wear loss characterizationThe dry sliding wear tests were conducted on a micro tribometer module, CETR UTM-2 operating with linear reciprocating motion drive. The samples are rubbed against a ball-shaped upper specimen made of 9.5 mm diameter tungsten carbide ball. A load of 25 N, stroke length of 2 mm, oscillation frequency of 5 Hz and test duration of 1000 seconds were selected for the operation. The dry sliding wear tests were carried out according to the ASTM G133-05 for determining the sliding wear of metals23. The wear
loss was calculated from the length of the stroke, the width of the wear scar and the depth of wear (groove) that were
made on the surface of the deposited samples as shown in equations (1) and (2)24.
Figure 2. SEM morphologies (a) Ti6Al4V powder; (b) Cu powder.
( ) sin
V L R WR W R W
W R W
3 3 1
l s p
d p d
= - - +
Wd Rp Rp W4 2
-Where Vl is the wear loss; Ls is the stroke length; Rp is the pitch radius; W is width of the wear scar and Wd represents the wear depth.
3. Results and Discussions
3.1. Microstructural analysis
The SEM analysis of the surface and the cross section of the parent material were characterised and the microstructures are shown in Figures 3 a-b.
Figure 3. SEM micrographs of the substrate (a) Surface; (b) Cross section.
The microstructures of the selected Ti6Al4V-3Cu and Ti6Al4V-5Cu alloys observed by SEM and Optical microscope (OM) are presented Figure 5.
The SEM analysis of sample Z1 of Ti6Al4V-5Cu alloy deposited with a laser power of 1200 W and scanning speed of 0.7 m/min is described in Figures 5 a-b with the Figure 5a showing the top view of the deposited alloy with the dominance of Widmanstätten structures. Figure 5b shows the middle view and the fusion zone (FZ) of the alloy. Here, the Widmanstätten structures were observed to be thinner towards to the FZ; and this was as a result of the heat sink that exists between the deposit and the substrate. Figures 5 c-d show the SEM analyses of sample Z2 of Ti6Al4V-3Cu alloy deposited with a laser power, a scanning speed and a
powder low rate of 1600 W, 0.3 m/min and 2.5 rpm; and
sample Z3 of Ti6Al4V-5Cu alloy deposited with a laser power and a scanning speed of 1200 W and 0.3 m/min; and their EDS analyses at the regions indicated by arrows. The black spots observed within the Widmanstätten structures were assumed to be oxides of titanium alloy. Figure 5e shows the microstructural analysis of sample Z2 of Ti6Al4V-3Cu alloy (deposited with a laser power and a scanning speed of 1600 W and 0.3 m/min) towards the top of the deposited alloy. Numerous erected, symmetrical and thick feathers-like microstructures were observed protruding from the grain boundaries and were elongated towards the top of the deposit of sample Z2. Figure 5f shows the OM analysis towards the substrate of sample Z3 of Ti6Al4V-5Cu alloy. Widmanstätten structures were observed in most of the microstructures and their textures are dependent on the process parameters used.
The -Ti phases were found to hinder the continuous low
(plastic deformation) of the -phase during cooling due to variation in the slip system. During this process, macroscopic banding is developed between the boundaries. Sample Z4 of Ti6Al4V-5Cu deposited with a laser power of 1400 W,
a scanning speed of 0.3 m/min and powder low rate of
2.4 rpm shows some backbone-like microstructure. The backbone-like structures were formed towards the top at an angle approximately 60o to the horizontal. -Ti lamella was
observed in gradient bundles between the backbone-like structures and the Widmanstätten structures.
3.2. The microhardness evaluation
The microhardness evaluation of the substrate and the deposited Ti6Al4V-Cu alloys are presented and discussed. Figure 6 displays the histogram plot of the microhardness values of the substrate (surface and cross section), Ti6Al4V alloy, Ti6Al4V-Cu, Ti6Al4V-3Cu and Ti6Al4V-5Cu alloys respectively.
The addition of Cu has greatly improved the microhardness values of Ti6Al4V alloy even though the hardness value of Ti6Al4V alloy was higher than 1 weight percent of Cu in Ti6Al4V-Cu alloy. The average microhardness values obtained
for the laser deposited Ti6Al4V alloy, Cu, Ti6Al4V-3Cu, and Ti6Al4V-5Cu are 444±49 VHN0.5, 397±56 VHN0.5, 547±16 VHN0.5, and 519±54 VHN0.5 respectively. The hardness measurements were conducted from the top of the deposit to the substrate and thereby solving for their average hardness values. Aoki et al.25 improved the mechanical properties of
cast Ti6Al4V alloy with the addition of (1 and 4) wt % Cu. Their hardness values were much improved as compared to the Ti6Al4V alloy25. It was so interesting that the hardness
of the alloys with 5 wt % of Cu was lower than that of the 3 wt % of Cu. However, it can also be construed that the density of Ti6Al4V-Cu alloys increases with an increase in Cu content. Ma et al.26 reported that a high density boundary
generates more plastic deformation that led to a decrease in material hardness26. Ti6Al4V alloy powder was deposited
on the substrate at a laser power of 1600 W and scanning speed of 0.3 m/min, and however its hardness values were measured in order to check for the hardness variation with that of the rolled Ti6Al4V alloy substrate. Thus, from the histogram plot, it was discovered that the hardness value of the laser deposited Ti6Al4V sample is more than the hardness value of the substrate (on both the surface and the cross section). This phenomenon is attributed to the heating and
cooling efect of the laser beam on the deposit. Thus, laser deposited Ti6Al4V alloy has a strong efect on the hardness
value compare with the rolled counterpart.
3.3. Tribological testing and the wear analysesThe results of the wear test conducted on the surfaces of the deposited alloys are presented and analysed. The back and forth movement of the tungsten carbide ball over the alloy’s surfaces has induced a wear ridge on them due to the high hardness of the wearing ball. An abrasive wear takes place between the carbide ball and the composites. Figures 7 a-d show the SEM micrographs of the worn surfaces of the substrate, Ti6Al4V alloy deposited at a laser power of 1600 W and scanning speed 0.3 m/min, Ti6Al4V-3Cu deposited at a laser power of 1600 W and scanning speed 0.3 m/min and Ti6Al4V-5Cu deposited at a laser power of 1200 W and scanning speed 0.3 m/min respectively.
Figure 6. Plot of microhardness of the substrate, Ti6Al4V alloy, Ti6Al4V-Cu, Ti6Al4V-3Cu and Ti6Al4V-5Cu alloys.
Figure 7. SEM micrographs of the worn surfaces of the alloys focused at low magniication (a) Substrate; (b) Ti6Al4V alloy; (c)
Ti6Al4V-3Cu; (d) Ti6Al4V-5Cu.
Ti6Al4V-Cu alloy. The diferent production processes of the
rolled substrate and the laser deposited Ti6Al4V alloy have
signiicant efect on their results. The size of ellipse sign
was reduced for Ti6Al4V-Cu composites and this could be
attributed to the Cu inclusion and the surface roughness of the composites. Figures 8 a-d show the SEM micrographs of the wear debris of the substrate, Ti6Al4V alloy, Ti6Al4V-3Cu and Ti6Al4V-5Cu alloys under the load of 25 N.
Figure 8. SEM micrographs of the worn surfaces (a) substrate; (b) Ti6Al4V alloy; (c) Ti6Al4V-3Cu; and (d) Ti6Al4V-5Cu.
the formation of debris particles in any sliding system and also the agglomeration due to the continuous rubbing of the two bodies. Although, the thermal conductivity (W/mK) of the tungsten carbide ball is 8 times than that of the Ti6Al4V alloy. The heat generated from the tungsten carbide will be induced into the Ti6Al4V alloy during rubbing. With the small amount of copper added, there is still an impact on the heat generated; and thus has enhanced the properties of
the Ti6Al4V-Cu alloy signiicantly. The total heat power
dissipated is equals to the work done by the friction force which is distributed between the two contacting bodies. It can also be stipulated that the substrate and Ti6Al4V
surfaces experiences a more signiicant abrasive wear under
the reciprocating sliding condition as compared to Ti6Al4V-3Cu and Ti6Al4V-5Cu alloys. During the rubbing action, particles of the titanium alloy are transferred and stuck to the tungsten carbide ball due to adhesion as a result of the heat generated. The magnitude of that adhesion depends on the load of 25N used, the speed of the rubbing ball and the condition of sliding (dry). Okabe et al.27 revealed that
the decrease in wear of Ti6Al4V is associated with the presence of Cu and feasibly the microstructures with the copper eutectoid in the crystal lattices improved the wear resistance as the ductility decreased. Conversely, the wear
resistance was further improved within the α+β alloy phase
to plastic deformation27. The substrate shows the lowest coeicient of friction, COF of 0.017, followed by the
Ti6Al4V with a COF of 0.035. The large width of wear track of the substrate majorly contributes to its low COF. Sample Z3 of Ti6Al4V-5Cu deposited at a laser power of 1200 W and scanning speed of 0.3 m/min was observed to have the highest COF of 0.05. This nature of rapid decrease of the COF has been reported by Xiong et al.28, though; their wear
analysis was conducted under distilled water. The loss of wear was calculated using the formular adopted by Qu and Truhan24. The width of wear, length of stroke and the wear
of depth has been applied to obtain the wear loss. Figure 9 presents the histogram plot of the wear loss.
Figure 9. Histogram plot of wear loss of the substrate, Ti6Al4V, and the Ti6Al4V-Cu alloys.
It can be detected that samples Z3, Z4 and Z5 of Ti6Al4V-5Cu alloys show the lowest percentage of wear losses of 0.162 mm3, 0.204 mm3 and 0.175 mm3 respectively; and
fell between 10 % and 14 %; but interestingly showed a higher COF as compared to the substrate. On the other hand, sample Z2 of Ti6Al4V-3Cu alloy depicts a percentage of 15 % which is slightly higher and possesses the wear loss of 0.236 mm3. The wear loss of the substrate and the
laser deposited Ti6Al4V alloy are 0.332 mm3 and 0.423
mm3 respectively. All the deposited Ti6Al4V-Cu alloys
showed an improvement in the wear resistance. Sample Z3 of Ti6Al4V-5Cu alloys deposited with the laser power of 1200 W and scanning speed of 0.3 m/min has the lowest wear loss. It was strangely fascinating that the wear loss of Ti6Al4V alloy is more than that of the substrate. Perhaps, the width and length of the wear scar of the substrate are more than that of the Ti6Al4V alloy but the depth is very much lower. In other word, the depth of wear and the width
of wear have a signiicant role to play in determining the
wear loss. The properties of Ti6Al4V-3Cu and Ti6Al4V-5Cu alloys are improved as compared with the substrate and the
Ti6Al4V alloy. Perpetually, the Cu ions have strengthened
the titanium lattices most especially the β-phases within the
body centred cubic region.
The surface modiication of Ti6Al4V alloy was achieved
through the addition of 3 wt% and 5 wt% of Cu through laser metal deposition process. The microhardness values of the Ti6Al4V-Cu alloys were improved when compared to the
substrate and Ti6Al4V alloys. The coeicient of friction of
the substrate and the Ti6Al4V alloy were lower than that of the Ti6Al4V-Cu alloys but the wear losses of both the Ti6Al4V-3Cu and Ti6Al4V-5Cu were greatly improved with a reduced plastic deformation. The substrate shows the widest in wear width and lowest in wear depth. The occurrence was envisaged to be due to the compressive nature of the grain boundaries and the rolled nature of the substrate. Sample Z3 of Ti6Al4V-5Cu alloys deposited with the laser power of 1200 W and scanning speed of 0.3 m/min has the lowest wear loss. Widmanstätten structures were detected in most of the microstructures and their textures are dependent on the process parameters used. The -Ti phases were found to
impede the continuous low (plastic deformation) of the
-phase during cooling due to variation in the slip system.
The authors would to acknowledge the Department of Mechanical Engineering, University of Johannesburg, South Africa and the inancial support from the Department of Defense through the research and educational program HBCU/MSI (contract # W911NF-15-1-0457) under the direct supervision of Dr. Joycelyn S. Harrison (Program Manager, AFOSR Complex Materials and Devices Program).
1. U.S. Congress, Oice of Technology Assessment. Advanced Materials by Design-Polymer Matrix Composite, OTA-E-351.
Washington: U.S. Government Printing Oice; 1988. p. 83-85.
2. Froes HF, Yau TL, Weidenger HG. Titanium, Zirconium and Hafnium. In: Matucha KH, ed. Materials Science and Technology - Structure and Properties of Nonferrous Alloys. Weinheim: VCH Verlag; 1996.
3. Boyer R, Welsch G, Collings EW, eds. Materials Properties Handbook: Titanium Alloys. Materials Park: ASM International; 1994. 1169 p.
4. Gogia AK, Nandy TK, Muraleedharan K, Banerjee D. The efect
of heat treatment and niobium content on the room temperature tensile properties and microstructure of Ti3Al-Nb alloys. Material Science and Engineering: A. 1992;159(1):73-86.
6. Okazaki Y, Ito Y, Ito A, Tateishi T. Efect of Alloying Elements
on Mechanical Properties of Titanium Alloys for Medical Implants. Materials Transactions, JIM. 1993;34(12):1217-1222.
7. Tian WH, Nemoto M. Efect of carbon addition on the microstructures and mechanical properties of γ-TiAl alloys.
8. Leyens C, Peters M, eds. Titanium and Titanium Alloys, Fundamentals and Applications. Weinheim: Wiley-VCH; 2003. 9. Structural Alloys Handbook. Columbus: Battelle’s Columbus
10. Fu Y, Loh NL, Batchelor AW, Liu D, Zhu X, He J, et al. Improvement in fretting wear and fatigue resistance of Ti–6Al–4V by application of several surface treatments and coatings. Surface and Coatings Technology. 1998;106(2-3):193-197.
11. Subramanian C, Cavallaro G, Winkelman G. Wear maps for titanium nitride coatings deposited on copper and brass with electroless nickel interlayers. Wear. 2000;241(2):228-233.
12. Ohkubo C, Shimura I, Aoki T, Hanatani S, Hosoi T, Hattori M, et al. Wear resistance of experimental Ti-Cu alloys. Biomaterials. 2003;24(20):3377-3381.
13. Al-Fozan SA, Malik AU. Efect of seawater level on corrosion behavior of diferent alloys. Desalination. 2008;228(1-3):61-67.
14. Al-Muhanna K, Habib K. Marine bio-fouling of diferent alloys exposed to continuous lowing fresh seawater by electrochemical
impedance spectroscopy. Journal of Saudi Chemical Society. 2016;20(4):391-396.
15. Legg M, Yücel MK, Garcia de Carellan I, Kappatos V, Selcuk C, Gan TH. Acoustic methods for biofouling control: A review. Ocean Engineering. 2015;103:237-247.
16. Sherif EM, Ammar HR, Khalil KA. Efects of copper and
titanium on the corrosion behavior of newly fabricated nanocrystalline aluminum in natural seawater. Applied Surface Science. 2014;301:142-148.
17. Wikispaces. Biological fouling in sea water coolant heat exchangers. Available from: <http://seawaterfouling.wikispaces. com/home>. Access in: 30/5/2017
18. Copper Development Association. Copper and its Alloys. Available from: <http://www.copperalliance.org.uk/copper-and-its-alloys/alloys/coppers>. Access in: 30/5/2017
19. Vijayan SR, Santhiyagu P, Ramasamy R, Arivalagan P, Kumar G, Ethiraj K, et al. Seaweeds: A resource for marine bionanotechnology. Enzyme and Microbial Technology. 2016;95:45-57.
20. ASTM International. ASTM E3-11 - Standard Guide for Preparation of Metallographic Specimens. West Conshohocken: ASTM International; 2011.
21. Struers. Application Note Titanium. Available from: <http:// www.struers.com/resources/elements/12/104827/Application_ Note_Titanium _English.pdf>. Access in: 15/10/2013.
22. ASTM International. ASTM E384 - 11e1 - Standard Test Method for Knoop and Vickers Hardness of Materials. West Conshohocken: ASTM International; 2011.
23. ASTM International. ASTM G133-05 (2016) - Standard Test Method for Linearly Reciprocating Ball-on-Flat Sliding Wear. West Conshohocken: ASTM International; 2016.
24. Qu J, Truhan JJ. An eicient method for accurately determining wear volumes of sliders with non-lat wear scars and compound
curvatures. Wear. 2006;261(7-8):849-855.
25. Aoki T, Okafor IC, Watanabe I, Hattori M, Oda Y, Okabe T. Mechanical properties of cast Ti6Al4V-XCu alloys. Journal of Oral Rehabilitation. 2004;31(11):1109-1114.
26. Ma CH, Huang JH, Chen H. Nanohardness of nanocrystalline
TiN thin ilms. Surface and Coatings Technology. 2006;200(12-13):3868-3875.
27. Okabe T, Kikuchi M, Ohkubo C, Koike M, Okuno O, Oda Y. The grindability and wear of Ti-Cu alloys for dental applications. JOM. 2004;56(2):46-48.